Visualizing Graphene Based Sheets by Fluorescence
Jaemyung Kim, Laura J. Cote, Franklin Kim, and Jiaxing Huang*
Department of Materials Science and Engineering, Northwestern UniVersity,
EVanston, Illinois 60208
Received August 9, 2009; E-mail: Jiaxingemail@example.com
Abstract: Graphene based sheets have stimulated great interest due to their superior mechanical, electrical,
and thermal properties. A general visualization method that allows quick observation of these single atomic
layers would be highly desirable as it can greatly facilitate sample evaluation and manipulation, and provide
immediate feedback to improve synthesis and processing strategies. Here we report that graphene based
sheets can be made highly visible under a fluorescence microscope by quenching the emission from a
dye coating, which can be conveniently removed afterward by rinsing without disrupting the sheets. Current
imaging techniques for graphene based sheets rely on the use of special substrates. In contrast, the
fluorescence quenching mechanism is no longer limited by the type of substrate. Graphene, reduced
graphene oxide, or even graphene oxide sheets deposited on arbitrary substrates can now be readily
visualized with good contrast for layer counting. Direct observation of suspended sheets in solution was
also demonstrated. The fluorescence quenching microscopy offers unprecedented imaging flexibility and
could become a general tool for characterizing graphene based materials.
Microscopy imaging techniques usually play a critical role
in material discoveries at small length scales. For example, the
discovery that graphene is visible under a normal optical
microscope when deposited on dielectric-coated silicon wafers1,2
has enabled numerous studies on these single atomic carbon
sheets.3-5 Graphene oxide (G-O)6,7 is a promising precursor
for solution processed, chemically modified graphene (a.k.a.
reduced G-O) thin films for applications such as flexible,
transparent conductors.8-10 Since the optical absorption of G-O
is much weaker than graphene,11 it is even more challenging to
visualize under optical microscope. Atomic force microscopy
(AFM) is often used to visualize G-O sheets since it gives
accurate thickness values on the nanometer scale.12 However,
it has not been made suitable for quick sample examination over
large areas due to rather low throughput. In addition, it typically
requires very smooth substrates, such as freshly cleaved mica
or silicon wafer. Scanning electron microscopy (SEM) can be
much faster, but it needs to operate under vacuum and works
best for films deposited on conducting substrates.13 High-
contrast optical imaging of G-O sheets has also been demon-
strated by interference technique14 and imaging ellipsometry,15
but only on dielectric-coated silicon wafers, where the thickness
of the dielectrics and the illuminating wavelength need to be
optimized. The need for special types of substrates to visualize
graphene based sheets greatly limits our capability to study these
new two-dimensional sheets. For example, solution processed
graphene films are found to be promising for flexible, transparent
plastic electronics. To establish how processing conditions affect
the final thin film quality, it is critical to see the microstructures
of the film to find out the size distribution of the sheets, the
coverage on the plastic substrate, and the degree of wrinkling
and overlapping. However, imaging graphene based sheets
deposited on plastic surface has been a great challenge with
current microscopy techniques. Therefore, alternative methods
that can image graphene based sheets without the need for
special substrates would be very useful for high-throughput
(1) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang,
Y.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. Science 2004,
(2) Novoselov, K. S.; Jiang, D.; Schedin, F.; Booth, T. J.; Khotkevich,
V. V.; Morozov, S. V.; Geim, A. K. Proc. Natl. Acad. Sci. U. S. A.
2005, 102, 10451–10453.
(3) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Katsnelson,
M. I.; Grigorieva, I. V.; Dubonos, S. V.; Firsov, A. A. Nature 2005,
(4) Gusynin, V. P.; Sharapov, S. G. Phys. ReV. Lett. 2005, 95, 146801.
(5) Wang, F.; Zhang, Y. B.; Tian, C. S.; Girit, C.; Zettl, A.; Crommie,
M.; Shen, Y. R. Science 2008, 320, 206–209.
(6) Li, D.; Kaner, R. B. Science 2008, 320, 1170–1171.
(7) Park, S.; Ruoff, R. S. Nat. Nanotechnol. 2009, 4, 217–224.
(8) Eda, G.; Fanchini, G.; Chhowalla, M. Nat. Nanotechnol. 2008, 3, 270–
(9) Tung, V. C.; Allen, M. J.; Yang, Y.; Kaner, R. B. Nat. Nanotechnol.
2009, 4, 25–29.
(10) Wang, X.; Zhi, L. J.; Mullen, K. Nano Lett. 2008, 8, 323–327.
(11) Li, D.; Muller, M. B.; Gilje, S.; Kaner, R. B.; Wallace, G. G. Nat.
Nanotechnol. 2008, 3, 101–105.
(12) Stankovich, S.; Dikin, D. A.; Piner, R. D.; Kohlhaas, K. A.;
Kleinhammes, A.; Jia, Y.; Wu, Y.; Nguyen, S. T.; Ruoff, R. S. Carbon
2007, 45, 1558–1565.
(13) Cote, L. J.; Kim, F.; Huang, J. X. J. Am. Chem. Soc. 2009, 131, 1043–
(14) Jung, I.; Pelton, M.; Piner, R.; Dikin, D. A.; Stankovich, S.;
Watcharotone, S.; Hausner, M.; Ruoff, R. S. Nano Lett. 2007, 7, 3569–
(15) Jung, I.; Vaupel, M.; Pelton, M.; Piner, R.; Dikin, D. A.; Stankovich,
S.; An, J.; Ruoff, R. S. J. Phys. Chem. C 2008, 112, 8499–8506.
Published on Web 12/04/2009
10.1021/ja906730d 2010 American Chemical Society260 9 J. AM. CHEM. SOC. 2010, 132, 260–267
sample evaluation in diverse applications. Here we report a
general method for visualizing graphene based sheets on
arbitrary substrates by fluorescence quenching microscopy
(FQM). The fluorescence quenching mechanism eliminates the
need for special substrates and even allows the direct observation
of graphene based sheets in solution. It offers unprecedented
imaging flexibility for characterizing graphene based materials.
A recent publication by Treossi et al.16 has shown that G-O
sheets can be visualized on glass, quartz, and silicon through
quenching the fluorescence of a thiophene dye covalently
tethered to the substrates. The current work presents an
enhancement because our FQM method can produce layer
contrast, does not involve surface functionalization thus allowing
observation on arbitrary substrates, and enables real-time
solution phase imaging.
Synthesis of Graphene, G-O, and Reduced Graphene
Oxide (r-G-O). Graphene was prepared by micromechanical
cleavage of highly oriented pyrolytic graphite using the “Scotch
Tape” method.1 G-O was synthesized using a modified Hummers
and Offeman’s method from graphite powder (Bay carbon,
SP-1).13,17,18 Chemically reduced graphene oxide (r-G-O) was
prepared by exposing G-O coated substrates to hot hydrazine vapor
(Sigma Aldrich, anhydrous, 98%) in a sealed chamber maintained
at 80 °C for overnight. Although all of these types of sheets were
successfully visualized, G-O sheets were used in most experiments
because they are much weaker absorbers and less effective
quenchers than r-G-O or graphene, and therefore represents a
“worst case” scenario for FQM imaging.
Solution Phase Fluorescence Quenching Measurement.
r-G-O water dispersion was prepared by hydrazine reduction of
G-O.9 Fluorescence spectra of fluorescent dye solutions were
acquired before and after adding minute aliquots of G-O or r-G-O
dispersions. The volume and concentration of G-O and r-G-O
dispersions added were kept the same. Three dyes with very
different molecular structures and absorption/emission profiles were
tested including a red fluorescent dye 4-(dicyanomethylene)-2-
methyl-6-(4-dimethylaminostyryl)-4H-pyran (DCM, Sigma-Aldrich,
98%), a green fluorescent dye fluorescein sodium salt (Sigma-
Aldrich), and a blue fluorescent dye 2,5-bis(5-tert-butyl-2-benzox-
azolyl)thiophene (BBOT, TCI America, >98%). The fluorescence
spectra were obtained by a photon counting spectrofluorimeter (ISS,
Sample Preparation. Glass microscope coverslips (VWR) and
SiO2/Si wafers were cleaned following the standard RCA treatment
method. Polyester substrates (Eppendorf) were cleaned with deion-
ized water. G-O film was deposited by Langmuir-Blodgett
technique13 (Nima Technology, Medium size LB deposition trough),
spin-coating (Laurell Technologies Corporation, WS-400, 1 min
at 4000 rpm), or drop casting. To improve the uniformity of the
dye coating, a polymer was codissolved with the dye for spin
coating. Typically, 1 mg of a green fluorescent dye-fluorescein
sodium salt powder was added to 10 mL of polyvinylpyrrolidone
(PVP, Sigma-Aldrich, MW ) 55 000)/ethanol solutions. Solutions
with 0.1, 0.5, 1, and 5 wt % of PVP were prepared to vary the
thickness of the coating. Since PVP forms a charge transfer complex
with fluorescein sodium salt at high polymer concentration,19 for
the 5 wt % PVP solution, 2 mg of dye powder were added to
compensate the fluorescence quenching by PVP (Figure S1 of the
Supporting Information). 100 µL of the coating solution was
dispensed for each 0.5 in2 of substrate area, and spun for 5 s at
300 rpm and then 45 s at 4000 rpm. The films produced from 0.5,
1, and 5 wt % of PVP solutions were measured to be approximately
10, 30, and 200 nm thick by surface profilometer (Veeco, Dektak
150), respectively. The thicknesses of films produced from 0.1 wt
% PVP solution were found to be smaller than 5 nm, although the
exact values were difficult to determine due to intrinsic surface
roughness of the coverslips. The dye/polymer film was also prepared
with resist materials that are commonly used in photolithography
and e-beam lithography for device fabrication